Journal of NanomaterialsVolume 2011 (2011), Article ID 432947, 5 pagesdoi:10.1155/2011/432947

Research Article

Preparation of Crystalline Sn-Doped TiO and Its Application in Visible-Light Photocatalysis

Zhou Xiufeng,¹ Lu Juan,¹ Li Lianghai,¹ and Wang Zuoshan1,2

¹College of Chemistry, Chemical Engineering and Materials Science, SooChow University, SooChow 215021, China²State Key Laboratory of Explosion Science and Technology, Beijing Institute of Technology, Beijing 100081, China

Received 21 June 2011; Revised 27 July 2011; Accepted 28 July 2011

Academic Editor: Chunyi Zhi

Copyright © 2011 Zhou Xiufeng et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

Sn-doped TiO₂ nanoparticles were prepared by the vapor transport method of water molecules and characterized by XRD and XPS analyses. The TEM images indicated that as-prepared samples were highly dispersed nanoparticles with a small and uniform size below 20 nm, as it would effectively control the rate of hydrolysis of Ti⁴⁺ by adjusting the flow speed of water vapor. Meanwhile, the photocatalytic properties of Sn-doped TiO₂ were tested, and the results showed that doping an appropriate amount of Tin would improve the photocatalytic activity of TiO₂ by enhancing the separation rate of photogenerated electrons and holes on the surface of TiO₂. In addition, the calcination temperature and Tin content had an important influence on the photocatalytic activity of TiO₂. When the mix ratio of Sn:Ti reached 1%, and the nano-Sn-TiO₂ sample was calcined at , it showed the best photocatalytic activity.

1. Introduction

TiO₂ has been considered as the most promising semiconductor photocatalyst [1–6] because of its high stability, low cost, and innocuity. However, it is only sensitive to UV light due to its large band gap (3.2 eV) [7], along with the relatively high electron-hole recombination rate [8, 9], which impedes its application. In order to use solar energy more efficiently, most of the investigations have been focused on preparing TiO₂ sensitive to visible light during the past several years [10–13]. Thus far, many ionic dopants in different valence states have been investigated, including both metallic ions (e.g., Ca²⁺, Sr²⁺, Ba²⁺, Al³⁺, Ga³⁺, Cr³⁺, Fe³⁺, Co³⁺, Ce³⁺, Ln³⁺, Sn⁴⁺, Zr⁴⁺, Nb⁵⁺, Mo⁵⁺, Sb⁵⁺ and Ta⁵⁺) and nonmetallic ions (e.g., N³⁺, C⁴⁺, S⁴⁺, F⁻, Cl⁻, and Br⁻) [14–17]. Particularly, TiO₂ doped with Sn has been proved to be an effective method and widely studied.

Preparations of Sn-doped TiO₂ photocatalysts focus on several methods such as sol-gel [18–21] and hydrothermal syntheses [22, 23], and chemical vapor deposition [24]. Among them, chemical vapor deposition needs special equipment. The other methods have a common ground that the reaction was performed in aqueous solution, and so, it is necessary for all of them to adjust the pH value of the solution to avoid rapid hydrolysis of Ti⁴⁺.

In this paper, Sn-doped TiO₂ was prepared by the vapor transport method of water molecules. It would effectively control the rate of hydrolysis of Ti⁴⁺ by adjusting the flow speed of vapor. In addition, isoamyl acetate was added as dispersant and it would be used circularly by spinning evaporation.

2. Experiments

2.1. Preparation of Sn-Doped TiO₂ Nanoparticles

In all experiments, deionized water was used. All of the chemical were analytical grade.

Sn-doped TiO₂ nanoparticles were prepared by water molecule transport method. Typically, 8 mL of tetrabutyl titanate, 40 mL of isoamyl acetate and 0.053 g of stannous chloride were mixed together in a flask. Air pump was turned on to transport air at a rate of 40 L·min⁻¹. A small quantity of water vapor was carried with the air from a beaker with water to the flask containing the mixture. Then, Ti⁴⁺ ions hydrolyzed slowly to form a white emulsion under ceaseless stirring for 1 h. After the reaction, isoamyl acetate was collected by spinning evaporation and used circularly. To obtain Sn-doped TiO₂ nanoparticles in which the mole ratio of Sn is about 1%, the precipitation was filtered, washed by distilled water, and sintered at 300–600°C for 2 h. Samples with different Sn proportions could be obtained by repeating the former steps, adding corresponding amount of stannous chloride. The Sn proportions mentioned here are all theoretical molar ratios of Sn:Ti in samples. The actual values were detected by EDS tests.

The pure and Sn-doped TiO₂ were designated as P-x and D-x, respectively, where “x” is the annealing temperature.

2.2. Characterization of the Samples

The crystalline phase was determined by X-ray diffraction (D/Max-IIIC, Shimadzu) instrument with Cu Kα radiation (λ = 0.15406 nm). The morphological feature and size of the product were observed by TEM (H600A-II, Hitachi). The analysis of element content of the doping system was done with XPS (ESCALAB 250, Thermo) and EDS (Quanta 200FEG, FEI) spectra. The photocatalytic activity of the samples was monitored on a 2550Z UV-Vis-NIR spectrophotometer.

2.3. Photocatalytic Activity

The photocatalytic activity of Sn-doped TiO₂ was evaluated by methylene blue degradation performed in XPA series instrument with a closed gas-circulating system and an inner irradiation quartz reactor. A 500 W xenon lamp was selected as the visible light source, and between the xenon lamp and reactor was inserted a cut filter (ZJB 420) to eliminate light of wavelength <420 nm. The flow rate of air was kept at a constant value of 500 mL·min⁻¹. In a typical experiment, 0.08 g of Sn-doped TiO₂ was dispersed in 250 mL of methylene blue (10 mg·L⁻¹) solution. The actual effect of photocatalytic activity by chemical reaction was studied by maintaining the solutions in dark for 1 h before irradiation. At given irradiation time intervals, the samples (5 mL) were taken out every 15 min and analyzed by UV-Vis spectrophotometer. The percentage of degradation was calculated via the formula (1−) × 100%, where A₀ is the absorbance of original methylene blue solution before irradiation and is the absorbance of methylene blue solution measured every 15 min in the process of photodegradation.

3. Results and Discussion

3.1. Characterization of Sn-Doped TiO₂ Nanoparticles

Figure 1 shows the XRD patterns for Sn-doped TiO₂ (1% for Sn) prepared with different annealing temperatures. The sample D-300 exhibits an anatase crystal structure (Figure 1(a)), while the sample D-600 is absolute rutile (Figure 1(d)). With increase of the annealing temperature, it turns to anatase gradually (Figures 2(b) and 2(c)). Hence, the lowest phase transition from anatase to rutile can take place at around 400°C for Sn-doped TiO₂, which is about 150°C lower than that for pure TiO₂ (550°C) [7]. No characteristic peaks of metal Sn or SnO₂ can be detected, because Sn was doped in TiO₂ in a small quantity and it was not enough to be detected.

Figure 1: XRD patterns of samples (Sn proportion is 1%) annealed at different temperatures(a) 300°C; (b) 400°C; (c) 500°C; (d) 600°C.

Figure 2: XRD patterns of samples with different Sn proportions annealed at 400°C (a) 0; (b) 0.5%; (c) 1%; (d) 5%.

The impact of different Sn proportions on the crystal phase of TiO₂ was investigated by XRD and the results were showed in Figure 2. Compared with the pure TiO₂ (Figure 2(a)), all of the Sn-doped TiO₂ ((Figures 2(b), 2(c), and 2(d)) annealed at 400°C exhibited rutile crystal structures partially, which further proved the doping of Sn would debase the phase transition temperature of TiO₂.

The average sizes of samples D-400 (containing Sn 0, 0.5, 1, 5%) are 7.9, 12.0, 8.9, and 8.2 nm estimated by Scherrer formula. The corresponding percentage () of rutile in the mixed crystal phase were 0, 25.3%, 27.9%, and 32.5%, calculated by the formula [25], where IA and IR are the diffraction peak intensity of anatase (2θ = 25.3°) and rutile (2θ = 27.4°), respectively. It was proved that more presence of Sn⁴⁺ facilitated the transformation of TiO₂ from anatase to rutile under the same temperature.

Figure 3 displays the TEM images of P-400 (Figure 3(a)), D-400, (Figure 3(b) and D-500 (Figure 3(c)). It could be observed that both P-400 and D-400 were nanoparticles with a uniform diameter of about 10 nm, implying doping Sn had no influences on the morphology and size of TiO₂. Sample D-500 was highly agglomerated with the particles of about 20 nm in size. It is consistent with the common sense that the crystal would grow bigger with the increase of the temperature.

(a)

(b)

(c)

Figure 3: TEM images of different samples: (a) P-400; (b) D-400; (c) D-500.

XPS analysis was performed to further study the existing states of Sn⁴⁺ in TiO₂. Figure 4 shows the survey spectrum of D-400 and inset is the Sn3d XPS spectrum. The doublet peak (486.4 and 494.8 eV) in the Sn3d XPS spectrum is ascribed to and of the substitutional Sn⁴⁺ dopants in the lattice, since the peak position of (486.4 eV) is located between that of SnO₂ (486.6 eV) and metallic Sn (484.4 eV) [26]. The radius of Sn⁴⁺ and Ti⁴⁺ ions are 0.071 and 0.068 nm, respectively. They are so close that it is easy for Sn⁴⁺ to replace Ti⁴⁺ in the lattice of TiO₂. The XPS analysis proved this perfectly.

Figure 4: XPS survey spectrum of Sn-doped TiO₂ nanocomposite.

The actual content of dopant Sn was tested by EDS analysis, and a typical EDS spectrum was showed in Figure 5 (D-400, Sn proportion is 0.5%, theoretically). Quantification of the EDS peaks gives the atomic ratios of Sn:Ti to be about 0.39%, 0.77%, and 3.34%, corresponding to the theoretical molar ratios of 0.5%, 1%, and 5%, respectively. It could be observed that there were some differences between the actual and theoretical values, mainly because some Sn was wasted in filter washing process. In addition, the quantification of the CO₂ absorbed on the surface of the samples was probably another reason.

Figure 5: The typical EDS pattern of Sn-doped TiO₂.

3.2. Photocatalytic Activity

We chose methylene blue (MB) as model dye to evaluate the photocatalytic activity of the photocatalysts under visible light irradiation, and the results were showen in Figures 6 and 7. Figure 6 showed the effects of the annealing temperature on the photodegradation of MB. As can be seen, the sample D-400 performed the best photocatalytic efficiency. On one hand, with the increase of the temperature, grain size increased and the specific surface area decreased, which is responsible for the depress of photocatalytic activity of Sn-doped TiO₂. On the other hand, under lower temperature, TiO₂ phase conversion was not sufficient, and it is difficult for Sn to dope into the TiO₂ lattice to form shallow electron traps, which resulted in the lower photocatalytic activity.

Figure 6: The effect of different annealing temperature on the degradation of MB under visible light.

Figure 7: The effect of different dosages of Sn⁴⁺ on the degradation of MB under visible light.

Figure 7 showed the effects of the different dosage of Sn⁴⁺ on the photodegradation of MB under visible light. Compared with the pure TiO₂ (sample P-400, Figure 6(a)), all of the samples D-400 exhibited a better photocatalytic activity. When tin dopant increases to 1% (Figure 6(c)), its photocatalytic activity reaches the maximum. Further increasing the tin dopant to 5% (Figure 6(d)) resulted in a decrease of its photocatalytic activity.

Photocatalytic activity mainly depended on the recombination rate of photogenerated electrons and holes produced in the course of photodegradation of MB under visible light. SnO₂ and TiO₂ are both wide band gap semiconductors. Although the band gap of SnO₂ (3.8 eV) is wider than that of TiO₂ (3.2 V), the Fermi lever of SnO₂ is lower than that of TiO₂ [27, 28]. It means that the photogenerated electrons may easily transfer from TiO₂ to SnO₂, but not to recombine with the photogenerated holes on the surface of TiO₂ immediately. Consequently, more and more holes are present on the surface and take part in the reactions of oxidizing OH⁻ and H₂O into hydroxyl radicals. Hydroxyl radicals would be finally responsible for the degradation of pollutants into H₂O and CO₂. Doping an appropriate amount of Tin would improve the photocatalytic activity of TiO₂, however, excessive amount of Sn⁴⁺ would induce the recombination of photogenerated electrons and holes, which resulted in the decrease of photocatalytic activity of TiO₂ [18].

4. Conclusion

Sn-doped TiO₂ nanoparticles were prepared by the water molecule transport method without adjusting the pH value of the solution. XRD results proved that the doping of Sn would debase the phase transition temperature of TiO₂. The effects of Sn dopant on the photocatalytic activity of TiO₂ nanoparticles were evaluated by the photodegradation of methylene blue under visible light. Results showed that doping an appropriate amount of Tin would improve the photocatalytic activity of TiO₂ by enhancing the separation rate of photogenerated electrons and holes on the surface of TiO₂. Among all of the samples, TiO₂ doped with 1% of Sn, annealed at 400°C, manifested the best photocatalytic activity.

References

J. Yuan, S. Zhou, L. Wu, and B. You, “Organic pigment particles coated with titania via sol-gel process,” Journal of Physical Chemistry B, vol. 110, no. 1, pp. 388–394, 2006.

R. J. James, G. Andrei, M. P. Laurence, S. Patrik, and B. W. Alison, “Dye-sensitized solar cells based on oriented TiO₂ nanotube arrays: transport, trapping, and transfer of electrons,” Journal of the American Chemical Society, vol. 130, no. 40, pp. 13364–13372, 2008.

G. H. Liu, Y. F. Zhu, X. R. Zhang, and B. Q. Xu, “Chemiluminescence determination of chlorinated volatile organic compounds by conversion on nanometer TiO₂,” Analytical Chemistry, vol. 74, no. 24, pp. 6279–6284, 2002.

S. Vaidyanathan, N. Zheng, E. G. Seebauer, and R. I. Masel, “Synthesis of high-temperature titania-alumina supports,” Industrial and Engineering Chemistry Research, vol. 45, no. 11, pp. 3815–3820, 2006.

S. Yuan, Q. R. Sheng, J. L. Zhang, H. Yamashita, and D. He, “Synthesis of thermally stable mesoporous TiO₂ and investigation of its photocatalytic activity,” Microporous and Mesoporous Materials, vol. 110, no. 2-3, pp. 501–507, 2008.

A. L. Linsebigler, G. Q. Lu, and J. T. Yates, “Photocatalysis on TiO₂ surfaces: principles, mechanisms, and selected results,” Chemical Reviews, vol. 95, no. 3, pp. 735–758, 1995.

Y. Q. Cao, T. He, L. S. Zhao, E. J. Wang, W. S. Yang, and Y. A. Cao, “Structure and phase transition behavior of Sn⁴⁺-doped TiO₂ nanoparticles,” Journal of Physical Chemistry C, vol. 113, no. 42, pp. 18121–18124, 2009.

Y. Q. Cao, T. He, Y. M. Chen, and Y. A. Cao, “Fabrication of rutile TiO₂-Sn/Anatase TiO₂-N heterostructure and its application in visible-light photocatalysis,” Journal of Physical Chemistry C, vol. 114, no. 8, pp. 3627–3633, 2010.

X. M. Song, J. M. Wu, M. Z. Tang, B. Qi, and M. Yan, “Enhanced photoelectrochemical response of a composite titania thin film with single-crystalline rutile nanorods embedded in anatase aggregates,” Journal of Physical Chemistry C, vol. 112, no. 49, pp. 19484–19493, 2008.

A. Dawson and P. V. Kamat, “Semiconductor-metal nanocomposites. Photoinduced fusion and photocatalysis of gold-capped TiO₂ (TiOa/Gold) nanoparticles,” Journal of Physical Chemistry B, vol. 105, no. 5, pp. 960–966, 2001.

R. Asahi, T. Morikawa, T. Ohwaki, K. Aoki, and Y. Taga, “Visible-light photocatalysis in nitrogen-doped titanium oxides,” Science, vol. 293, no. 5528, pp. 269–271, 2001.

S. Sakthivel and H. Kisch, “Daylight photocatalysis by carbon-modified titanium dioxide,” Angewandte Chemie, vol. 42, no. 40, pp. 4908–4911, 2003.

W. Macyk and H. Kisch, “Photosensitization of crystalline and amorphous titanium dioxide by platinum(IV) chloride surface complexes,” Chemistry, vol. 7, no. 9, pp. 1862–1867, 2001.

O. Carp, C. L. Huisman, and A. Reller, “Photoinduced reactivity of titanium dioxide,” Progress in Solid State Chemistry, vol. 32, no. 1-2, pp. 33–177, 2004.

A. Kitiyanan, S. Ngamsinlapasathian, S. Pavasupree, and S. Yoshikawa, “The preparation and characterization of nanostructured TiO₂-ZrO₂ mixed oxide electrode for efficient dye-sensitized solar cells,” Journal of Solid State Chemistry, vol. 178, no. 4, pp. 1044–1048, 2005.

M. Dürr, S. Rosselli, A. Yasuda, and G. Nelles, “Band-gap engineering of metal oxides for dye-sensitized solar cells,” Journal of Physical Chemistry B, vol. 110, no. 43, pp. 21899–21902, 2006.

J. Li and H. C. Zeng, “Hollowing Sn-doped TiO₂ nanospheres via Ostwald ripening,” Journal of the American Chemical Society, vol. 129, no. 51, pp. 15839–15847, 2007.

J. Sun, X. L. Wang, J. Y. Sun, R. X. Sun, S. P. Sun, and L. P. Qiao, “Photocatalytic degradation and kinetics of Orange G using nano-sized Sn(IV)/TiO₂/AC photocatalyst,” Journal of Molecular Catalysis A, vol. 260, no. 1-2, pp. 241–246, 2006.

X. Li, R. C. Xiong, and G. Wei, “Preparation and photocatalytic activity of nanoglued Sn-doped TiO₂,” Journal of Hazardous Materials, vol. 164, no. 2-3, pp. 587–591, 2009.

L. Q. Jing, H. G. Fu, B. Q. Wang, et al., “Effects of Sn dopant on the photoinduced charge property and photocatalytic activity of TiO₂ nanoparticles,” Applied Catalysis B, vol. 62, p. 282, 2006.

S. Mahanty, S. Roy, and S. Sen, “Effect of Sn doping on the structural and optical properties of sol-gel TiO₂ thin films,” Journal of Crystal Growth, vol. 261, no. 1, pp. 77–81, 2004.

J. Liu, Y. Zhao, L.Y. Shi, et al., “Solvothermal synthesis of crystalline phase and shape controlled Sn⁴⁺-doped TiO₂ nanocrystals: effects of reaction solvent,” Applied Materials & Interfaces, vol. 3, no. 4, pp. 1261–1268, 2011.

E. Arpaç, F. Sayılkan, M. Asiltürk, P. Tatar, N. Kiraz, and H. Sayılkan, “Photocatalytic performance of Sn-doped and undoped TiO₂ nanostructured thin films under UV and vis-lights,” Journal of Hazardous Materials, vol. 140, no. 1-2, pp. 69–74, 2007.

Y. A. Cao, W. S. Yang, W. F. Zhang, G. Z. Liu, and P. Yue, “Improved photocatalytic activity of Sn⁴⁺ doped TiO₂ nanoparticulate films prepared by plasma-enhanced chemical vapor deposition,” New Journal of Chemistry, vol. 28, no. 2, pp. 218–222, 2004.

S.-W. Yang and L. Gao, “Simple and effective preparation of N-doped TiO₂ nanocrystallites with visible-light activities,” Journal of Inorganic Materials, vol. 20, no. 4, pp. 785–788, 2005.

J. Wang, W. Wu, and D. Feng, The Introduction of Electronic Spectroscopy, The Publishing House of Defense Industry, Beijing, China, 1992.

B. F. Xin, D. D. Ding, Y. N. Gao, X. G. Jin, H. Fu, and P. Wang, “Preparation of nanocrystalline Sn-TiO₂-X via a rapid and simple stannous chemical reducing route,” Applied Surface Science, vol. 255, no. 11, pp. 5896–5901, 2009.

F. Sayılkan, M. Asiltürk, P. Tatar, N. Kiraz, E. Arpaç, and H. Sayılkan, “Photocatalytic performance of Sn-doped TiO₂ nanostructured mono and double layer thin films for Malachite Green dye degradation under UV and vis-lights,” Journal of Hazardous Materials, vol. 144, no. 1-2, pp. 140–146, 2007.